Standard Test Method for Determining the Consistency of Refractory Castable Using the Ball-In-Hand Test
This method determines the optimum water content and consistency of castable products. Consistency is judged with the Ball-in-Hand method or measured with the Flow Table method.
SIGNIFICANCE AND USE
This test method is used primarily to determine if a freshly mixed refractory castable is of the proper consistency and therefore would most likely provide optimum performance. It can also be used to estimate the correct water addition rate of a castable when either the manufacturer's specified water content is not available or when unique circumstances have rendered that recommendation unusable.
The correct water content is an important factor that must be controlled to obtain optimum castable performance. Excess water can reduce strength, increase volume shrinkage, and promote segregation of the castable ingredients. Insufficient water can produce "honeycombs" (air voids) in the castable because of the insufficient mobility during placement and in extreme cases can prevent the complete hydration of the cement (if used).
The Ball-in-Hand test is subjective and somewhat depends on the skill of the operator. However, it is a universally accessible method due to the simplicity of the equipment required, and it is readily used in the field.
The total wet mixing time of a castable influences the rheological and final properties and therefore should be monitored.
This test method can be performed in a laboratory or on a job site.
This test method is not intended to determine the proper consistency for gunning applications, although it may provide information of value for interpretation by a skilled operator.
1.1 This test method covers the procedures for determining the consistency of a castable using the Ball-in-Hand Test. The amount of water used in a castable has a significant influence on its performance.
1.2 This test method applies to regular weight castable refractories and insulating castable refractories which are described in Classification C401. It also applies to such castables containing metal fibers.
1.3 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. (See 6.2.3 for a specific safety warning.)
Extracted, with permission, from ASTM C860 Standard Test Method for Determining the Consistency of Refractory Castable Using the Ball-In-Hand Test, copyright ASTM International, 100 Barr Harbor Drive, West Conshohocken, PA 19428. A copy of the standard may be purchased from ASTM International, phone 610-832-9555, e-mail: email@example.com, website: www.astm.org.
FROM THE BLOG...
Orton's 2019 "Introduction to Refractories" short course is coming up in August. This course is an intensive...
01/18/2019New Laboratory Training Course Announced
LABORATORY TRAINING - THERMAL PROPERTIES OF REFRACTORIES - March 19, 20 & 21, 2019 A Three Day Course...
ADVANCED THERMAL PROPERTIES OF REFRACTORIES - October 29 & 30, 2018 A Two Day Course Sponsored by...